Comparison of Wear Rate between Ceramic-on-
Ceramic, Metal on Highly Cross-linked Polyethylene, and Metal-on-Metal Bearings
Comparação da taxa de desgaste entre componentes de cerâmica sobre cerâmica, metal sobre polietileno de alta ligação cruzada e metal sobre metal
1Department of Orthopedic Surgery, Nagoya University Graduate School of Medicine, Tsurumai-cho, Showa-ku Nagoya, Japan Rev Bras Ortop 2019;54:295–302.
Address for correspondence Yoshitoshi Higuchi, Department of Orthopedic Surgery, Nagoya University Graduate School of Medicine, 65 Tsurumai-cho, Showa-ku Nagoya, Japan 466-8550
Currently, there is a lack of evidence on the medium-term follow-up of cementless total hip arthroplasty (THA) using metal on highly cross-linked polyethyl- ene (MoP), ceramic-on-ceramic (CoC), and metal-on-metal (MoM) bearings. Our aim was to calculate the 5- to 10-year wear rate and the incidence rate of osteolysis for 3 types of bearings.
A total of 77 patients underwent MoP, 105 underwent ceramic CoC, and 55 underwent MoM THAs. The average patient age at the time of surgery was 64.7, 55.9, and 59.9 years old in the MoP, CoC, and MoM bearings, respectively. Clinical and radiologic measurements at a mean follow-up of 7.6 years were analyzed.
The mean postoperative Harris hip scores showed no difference among the groups. The mean annual liner wear rates were 0.0160, 0.0040 and 0.0054 mm/year in MoP, CoC bearings, and MoM bearings, with that of CoC bearings being signiﬁ
cantly lower than the others. Osteolysis (14.5%) among MoM bearings was signiﬁ
cantly more frequently observed compared with the others. Kaplan-Meier survival at 10 years with implant loosening, or revision THA as the endpoint, was 96.1% (95% conﬁ
dence interval [CI]: 88.4–
98.7) for MoP, 98.6% (95% CI: 90.3–
98.6) for CoC bearing, and 98.2% (95% CI:
99.7) for MoM bearings (p¼
Excellent clinical and radiological outcomes were obtained for MoP and CoC bearings.
The present study was conducted at the Department of Orthopedic Surgery of the Nagoya University Graduate School of Medicine, Tsurumai-cho, Showa-ku Nagoya, Japan.
Yoshitoshi Higuchi’s ORCID is https://orcid.org/0000-0002-1112- 2682.
received January 19, 2018 accepted July 10, 2018
Copyright © 2019 by Sociedade Brasileira de Ortopedia e Traumatologia. Published by Thieme Revnter Publicações Ltda, Rio de Janeiro, Brazil
Total hip arthroplasty (THA) for patients with end-stage osteoarthritis of the hip aims at ensuring long-lasting pain relief.1,2 However, despite improved implant designs and surgical techniques, aseptic loosening and osteolysis due to particulate debris, generated from conventional polyethyl- ene, have become major limitations to long-term survival of prosthetics.3–6Osteolysis has been reported in up to 60% of young, active patients with conventional polyethylene.6In an attempt to avoid problems caused by wear-related debris, various types of bearing surfaces have been designed, such as metal on highly cross-linked polyethylene (MoP), a bearing- surface interaction with reduced linear and volumetric wear in comparison with conventional polyethylene.3,4,6,7 Simi- larly, hard bearing surfaces, which ensure even lower levels of volumetric wear, such as ceramic-on-ceramic (CoC) and metal-on-metal (MoM), have also been developed to address the problem of osteolysis.
However, they have their own inherent limitations, such as ceramic fractures and squeaking, or adverse local tissue reac- tion (ALTR).1,2,6,8Over the last 2 decades, several systematic reviews and many clinical randomized controlled trials com- paring the survivorship of THA implants with different bearing
surfaces have been published. However, the results of these studies are inconsistent and continue to be debated.2,6,8–11
Therefore, the aim of our study was to perform a retro- spective evaluation of the clinical and radiographic outcomes between MoP, CoC, and MoM cementless THAs over a 5- to 10-year follow-up period to compare the wear rates and the incidence of osteolysis.
Between August 2007 and December 2011, we performed consecutive primary CoC, MoP, or MoM THAs, with the type selected based on the recommendation of the senior surgeon performing the procedure. In total, 220 patients (237 THAs), who completed a minimum follow-up period of 5 years, were eligible for the present study. The exclusion criteria were:
death from causes unrelated to surgery (one patient; one joint), patient inaccessibility (ﬁve patients moved abroad;
ﬁve joints) and Crowe group III/IV hips (three patients; three joints). No signiﬁcant differences were noted between the groups with regard to gender, body mass index (BMI), or diagnosis (►Table 1). However, the age of the patients at the time of the surgery for the group who received CoC THAs was
Hoje, não há evidências sobre o acompanhamento em médio prazo da artroplastia total do quadril não cimentada com componentes de polietileno de alta ligação cruzada (highly cross-linked) sobre metal, cerâmica sobre cerâmica e metal sobre metal. Nosso objetivo foi calcular a taxa de desgaste em 5 a 10 anos e a taxa de incidência de osteólise nos três tipos de componentes.
Setenta e sete pacientes foram submetidos à artroplastia total de quadril com componentes de polietileno de alta ligação cruzada sobre metal, 105 foram submetidos ao mesmo procedimento com componentes de cerâmica sobre cerâmica e 55 foram submetidos à artroplastia total quadril com componentes de metal sobre metal. A média de idade dos pacientes no momento da cirurgia foi de 64,7, 55,9 e 59,9 anos nos grupos de componentes de polietileno de alta ligação cruzada sobre metal, cerâmica sobre cerâmica e metal sobre metal, respectivamente. As medidas clínicas e radiológicas em um período médio de acompanhamento de 7,6 anos foram analisadas.
As pontuações médias de Harris no período pós-operatório não mostra- ram diferença entre os grupos. As taxas médias anuais de desgaste do revestimento foram de 0,0160, 0,0040 e 0,0054 mm/ano em componentes de polietileno de alta ligação cruzada sobre metal, cerâmica sobre cerâmica e metal sobre metal; a taxa de desgaste dos componentes de cerâmica sobre cerâmica foi signiﬁ
cativamente menor do que as demais. A osteólise (14,5%) nos componentes de metal sobre metal foi signiﬁ
cativamente mais frequente em comparação aos demais. A sobrevida de Kaplan- Meier aos 10 anos com afrouxamento do implante ou revisão da artroplastia total do quadril como desfecho foi de 96,1% (intervalo de conﬁ
ança de 95% [IC95%]: 88,4–
98,7) nos componentes de polietileno de alta ligação cruzada sobre metal, 98,6% (IC95%:
98,6) nos componentes de cerâmica sobre cerâmica e 98,2% (IC95%: 88,0–
99,7) nos componentes de metal sobre metal (p¼
Os resultados clínicos e radiológicos de componentes de polietileno de alta ligação cruzada sobre metal e cerâmica sobre cerâmica foram excelentes.
signiﬁcantly lower than that of the other groups. Informed consent was obtained from all of the patients, and the present study was approved by the ethics committee of our hospital.
A posterolateral approach was used for all procedures, with patients in the lateral decubitus position. The socket wasﬁxed in the acetabulum using an acetabular alignment guide, with a target acetabular position of 20° of anteversion and 45° of inclination.12
Acetabular and Femoral Components
Acetabular and femoral components used for MoP and CoC THAs were manufactured by Stryker Orthopaedics (Mahwah, NJ, USA), while those for MoM were from Depuy Orthopae- dics (Warsaw, IN, USA) (►Fig. 1and►Table 1). The Crossﬁre Polyethylene Insert (Stryker Orthopaedics) was used for all cases in which a highly cross-linked polyethylene liner was implanted, with the BIOLOX forte (Ceramtec, Plochingen, Germany) used as a ceramic liner and head. The diameter of
the cobalt chrome head and of the ceramic head used is provided in►Table 1.
The clinical data of the patients, including the Harris hip score (HHS), were prospectively recorded by a senior surgeon 1 month prior to the THA, at 6 months and 1 year post-THA, and then annually, up to the endpoint of the follow-up. These data were then retrospectively extracted from the medical records of the patients for analysis.
Radiographs of the hips were obtained in the standard anteroposterior (AP) view, with both hips in neutral rotation and 0° abduction, and in the Lauenstein (frog position) view, with the patient in the supine position and the hips in 45°
abduction.7,13Radiographs were obtained at 3 months post- operatively and then annually until the last follow-up.
Deﬁnite loosening of the femoral component was deﬁned as a progressive axial subsidence of>3 mm or a varus or valgus shift.14 Deﬁnite loosening of the acetabular component was Table 1 Patient demographics
Age (years old) (range) 64.79.7
Gender (male/female) 9/68 20/85 11/44 0.320
Body mass index (kg/m2) (range) 23.13.2 (15.6–31.2)
Follow up (years) (range) 7.01.0 (5–10)
Diagnosis (n, %) 0.769
Osteoarthritis 73 (94.8%) 93 (88.6%) 50 (90.9%)
Avascular necrosis 4 (5.2%) 11 (10.5%) 5 (5.1%)
Post-traumatic osteoarthritis 0 1 (0.9%) 0
Implants Cementless Cup
Trident PSL 24 (31.2%) 22 (21.0%) NA
TriAD HA 53 (68.8%) 74 (70.5%) NA
Secur Fit AD NA 9 (8.5%) NA
Pinnacle-A NA NA 55 (100%)
Super Securﬁt HA 77 (100%) 105 (100%) NA
G2 stem NA NA 55 (100%)
Fomoral head diameter
22 mm 7 (9.1%) NA 0
26 mm 70 (91.9%) NA 0
28 mm 0 67 (63.8) 28 (50.9%)
32 mm 0 38 (36.2) NA
36 mm 0 0 27 (49.1%)
Abbreviations: BMI, Body mass index; CoC: ceramic-on-ceramic; MoM: metal-on-metal; MoP: metal on highly cross-linked polyethylene; NA, Not available. All of the values are given as the mean and standard deviation.
CoC THAs vs MoM THAsp<0.001.
†CoC THAs vs MoP THAsp<0.001.
deﬁned as a change in the vertical and/or medial position of
>2 mm or as the presence of a continuous radiolucent line>2 mm in width on both AP- and Lauenstein-view radiographs.15 Osteolysis was deﬁned as areas of endosteal, intracortical or cancellous bone destruction of>2 mm, which were non-linear and progressive.16 The acetabular inclination was measured using the transischial line as a reference, and anteversion was measured from digitized AP radiographs, using the method of Lewinnek et al.17Using the methods of Dorr et al apud Barrack et al,18the penetration of the femoral head into the liner was measured from digitized AP- and Lauenstein-view radiographs (►Fig. 2) by two surgeons using the Roman software, Version 1.70 (Institute of Orthopaedics, Oswestry, UK).
The femoral head penetration was measured at annual intervals to calculate the rate of wear, true wear and creep.
The true wear represented the steady-state linear wear rate, while creep represented a measure of early head penetration, a feature attributable to the so-called“running-in”wear, in cases involving hard-on-hard bearings, or polyethylene creep and deformation in cases involving MoP.5The wear rate was calcu- lated by dividing total femoral head penetration at the end- point of observation by the number of years of follow-up. Linear regression models of femoral head penetration over time were constructed, with the y-intercept representing the creep rate or
“running-in,” and the slope of the line representing the true wear rate.11,19 Intraclass correlation coefﬁcients (ICCs) were calculated and used to determine interobserver reliability regarding the measurement of femoral head penetration. In the MoM group, patients underwent magnetic resonance im- aging (MRI) when indicated, based on clinical symptoms, including hip pain or discomfort of the hip and concern for ALTR.
Statistical analyses were performed using SPSS Statistics for Windows, Version 21 (IBM Corp., Armonk, NY, USA) and EZR (Saitama Medical Center, Jichi Medical University, Tochigi,
Japan). The differences between the groups were evaluated using analysis of variance (ANOVA), the Tukey test, the Pearson chi-squared test, the Holm-Bonferroni methods, and the log- rank test, as appropriate. Ap-value<0.05 was considered statistically signiﬁcant.
The mean postoperative HHS was 85.3, 89.9, and 90.3 among cases involving MoP, CoC, and MoM THAs, respectively (p¼0.063) (►Table 2). Neither the incidence of dislocation nor the heterotopic bone formation differed among the three groups (►Table 3). All of theﬁve dislocations were successfully treated conservatively via single closed reduction, without recurrence. All of the joints were classiﬁed as Brooker class 120 with the patients showing no symptoms. There was no ceramic fracture among cases involving CoC THAs (►Table 3).
One joint among those having undergone MoP THAs (1.3%) required a revision THA owing to aseptic loosening of the cup. One joint (0.9%) among those having undergone CoC THAs required a revision THA owing to progressive femoral osteolysis caused by femoral neck impingement on the elevated acetabular metal liner. No cases of revision THA was observed among those involving MoM THAs.
One joint (0.9%) among those involving CoC THAs exhib- ited audible squeaking; however, a revision THA was not required because the condition was painless. No incidence of deep infection or of pulmonary embolism was identiﬁed in either group. One incidence of deep vein thrombosis (DVT) was identiﬁed among the cases involving MoP THAs; how- ever, no DVT was observed in the CoC and MoM THA groups.
Based on the Kaplan-Meier survival curve analysis, con- sidering implant loosening or revision THA as the endpoint, at 10 years, prosthetic survival was 96.1% (95% conﬁdence interval [CI]: 90.0–99.3) for the MoP group, 98.6% (95% CI:
Fig. 1 Cementless components used in the present study. (A) Metal on highly cross-linked polyethylene bearing. (B) Ceramic-on-ceramic bearing. (C) Metal-on-metal bearing.
90.3–98.6) for the CoC group, and 98.2% (95% CI: 88.0–99.7) for the MoM THA group. These values were not signiﬁcantly different among the groups (p¼0.360)
Neither the anteversion nor the inclination of the implanted acetabular component differed between the three THA groups (►Table 2). The incidence rate of osteolysis was greater for MoM THAs than either MoP (p<0.05) or CoC (p<0.001) THAs (►Table 3). Although no joints among CoC THAs showed aseptic loosening, 2 joints (2.6%) among MoP THAs showed loosening, with 1 of these cases (1.3%) requir- ing revision because of progression of loosening. In contrast, 1 joint (1.8%) among MoM THAs showed aseptic cup loosen- ing (►Table 3). Magnetic resonance imaging was performed on a total of 10 hips (18.2%). A pseudocystic tumor was identiﬁed in four hips; as the symptoms were minimal, a revision THA was not required.
The Wear Rate
Femoral head penetration could not be measured in eight joints among patients with CoC THAs, and in two joints among
patients with MoM THAs because the margin of the femoral head could not be identiﬁed clearly in these joints. Thus, measures of femoral head penetration were obtained for 97 and 53 joints among patients with CoC and MoM THAs, respectively. The ICC of measurement was 0.737 (95% CI:
0.16–0.982;p¼0.0043) for CoC, 0.876 (95% CI: 0.490–0.977;
p¼0.002) for MoP, and 0.761 (95% CI: 0.203–0.958;p¼0.001) for MoM THAs.
The wear rates of CoC and MoM THAs were signiﬁcantly lower than that of MoP THAs, irrespective of the radiographic view (AP and Lauenstein,p<0.0001). In addition, the wear rate was signiﬁcantly lower for CoC than for MoM THAs on AP- view radiographs, while the wear rate in the Lauenstein-view showed no difference between CoC and MoM THAs (►Table 4).
The running-in rate for CoC THAs was of 0.0036 mm/year based on AP radiographs, and of 0.0028 mm/year based on Lauenstein-view radiographs. The running-in rate for MoM THAs was of 0.0013 mm/year based on AP radiographs and of 0.0018 mm/year based on Lauenstein-view radiographs. Con- versely, the creep rate for MoP THAs was of 0.0426 mm on AP- view radiographs and of 0.0440 mm on Lauenstein-view radiographs (►Fig. 3). The true wear rate for MoP THAs was Fig. 2 Digitized anteroposterior view radiographs using the computer-digitizer facilities of the Roman software, Version 1.70 (Institute of Orthopaedics, Oswestry, UK) were obtained to determine femoral head penetration into the liners. (A) Metal on highly cross-linked polyethylene bearing. (B) Ceramic-on-ceramic bearing. (C) Metal-on-metal bearing.
of 0.0096 mm/year on AP-view radiographs and of 0.0093 mm/
year on Lauenstein-view radiographs, while the rate for CoC was of 0.0037 mm/year on AP-view radiographs and of 0.0038 mm/year on Lauenstein-view radiographs. Conversely, the true wear rate for MoM THAs was of 0.0051 mm/year on AP- view radiographs and of 0.0050 mm/year on Lauenstein-view radiographs.
The main reason for failure of THA with conventional poly- ethylene is wear of the bearing surface and the resultant
wear-induced osteolysis, which can result in implant loos- ening and failure.8,9,21 Therefore, modern materials with improved wear characteristics, such as metal, ceramics, and highly cross-linked polyethylene, have been implanted worldwide for use in THA.9,21–23
Previous studies have shown that survival with aseptic loosening at the midterm follow-up does not differ signiﬁ- cantly between CoC and MoP THAs.6,10However, few studies have compared midterm outcomes between MoP, CoC, and MoM THA, without a meta-analysis being available.24In our study, we have found that the survival rates at the 10-year follow-up with regard to implant loosening or revision THA did not differ signiﬁcantly between the three types of THAs.
However, the risk of osteolysis was signiﬁcantly higher with MoM than with CoC and MoP THAs. Therefore, the revision rate of MoM THA in long-term follow-up may be higher than that of the other THAs, because of gradually increasing osteolysis with the passage of time.25
Previous studies reported a mean liner wear rate of between 0.01 and 0.059 mm/year for MoP THAs, measured using AP radiographs.5,6,26,27 In contrast, the mean liner wear rate for CoC THAs was of between 0.00183 and 0.0067 mm/year based on AP radiographs.6,28The in vitro wear rate of CoC and MoM components were of<0.1 mm3/ million cycles and of<1.0 mm3/million cycles, respective- ly.29 Thus, our results are fairly consistent with those of previous reports in that the wear rate for CoC THAs was roughly 25% of the rate for MoP THAs. The wear rate for MoM THAs wasone-third of that for MoP THAs.
The true wear rate for MoP THAs was previously reported to be of 0.006 mm/year.19 However, to the best of our Table 2 Clinical and radiographicﬁndings
Preoperative 57.09.7 59.99.2 61.210.5 0.067
Last follow-up 87.08.0 89.97.3 90.37.1 0.054
Acetabular component position
Anteversion (°) 20.75.5 17.46.9 19.63.1 0.059
Inclination (°) 46.95.5 45.95.5 45.13.1 0.158
Overall 2 (2.6%) 2 (1.9%) 8 (14.5%) ‹0.001†
Acetabular 2 (2.6%) 1 (0.9%) 5 (9.1%) 0.016‡
Femoral 1 (1.3%) 2 (1.9%) 4 (7.3%) 0.143
Overall 2 (2.6%) 0 1 (1.8%) 1
Cup 1 (1.3%) 0 1 (1.8%) 1
Stem 1 (1.3%) 0 0 1
Abbreviation: CoC: ceramic-on-ceramic; HHS, Harris hip score; MoM: metal-on-metal; MoP: metal on highly cross-linked polyethylene. All of the values are given as the mean and standard deviation.
CoC THAs vs MoM THAs:p<0.001.
†MoM THAs vs MoP THAs:p<0.05.
‡CoC THAs vs MoM THAs:p<0.05.
Table 3 Complications
Parameters MoP (n¼77)
Revision THA 1 (1.3%) 1 (0.9%) 0 0.598 Deep joint
0 0 0 1
Dislocation 2 (2.6%) 2 (1.9%) 1 (1.8%) 0.797
DVT,PE 1 (1.3%)/0 0/0 0/0 0.556
4 (5.2%) 2 (1.9%) 2 (3.6%) 0.138
NA 0 NA
Abbreviation: CoC: ceramic-on-ceramic; DVT, Deep vein thrombosis;
MoM: metal-on-metal; MoP: metal on highly cross-linked polyethylene;
PE, Pulmonary embolism; THA, Total hip arthroplasty.
knowledge, the true wear rate for MoM THAs has not been reported thus far. The true wear rate of CoC THAs, as per our previous study, was50% of that of MoP THAs.
The overall THA survivorship was high for all of the groups, with no signiﬁcant differences between the groups.
The wear rates of MoM and CoC THAs were signiﬁcantly lower than that of MoP THAs. However, MoM THAs exhibited more frequent osteolysis and demonstrated a signiﬁcantly higher risk of revision compared with CoC and MoP THAs.24 Thus, excellent clinical and radiological outcomes were obtained for CoC and MoP THAs. Longer-term studies are needed to determine the effect of the wear rate and true wear rate on implant longevity.
The present study has some limitations. First, our study is retrospective in nature, with a relatively small number of patients. Also, the analysis was based on consecutive cases, with no randomization and no power analysis performed to determine if sufﬁcient patients were included to detect clinically meaningful differences between groups. The patients who received CoC THAs were signiﬁcantly younger than the patients in the other groups. This might have been caused by selection bias and might have affected the clinical
and radiographic results. Second, we have measured femoral head penetration using the technique described by Dorr et al along with the computer-digitizer facilities of the Roman software, Version 1.70. The validity of this method for measuring femoral head penetration following CoC THAs has been previously reported.6,11,19However, validation of MoM THA has never been reported. This method, which is typically used to examine femoral head penetration follow- ing MoP THA, is not easily applicable for CoC and MoM THAs.
Third, we could not analyze the metal artifact reduction sequence MRI and serum metal ion levels for all of the patients with MoM THAs and could not identify an objective causative factor of osteolysis. Further studies are needed to clarify the association between bearing type and osteolysis.
Finally, there were major differences in relation to the diameter of the prosthetic heads used in the three groups.
In a hip simulator study, the wear rate of 36-mm ceramic bearings was signiﬁcantly higher than that of 28-mm bear- ings, owing to their larger contact area, and paucity of lubrication when subjected to edge loading conditions.29 This suggests the possibility of increased wear with the use of large heads in certain circumstances.
Table 4 Wear rate
Wear rate (mm/year)
AP view 0.01610.0051 0.00410.0022 0.00540.0019 ‹0.001‡,§,¶
Lauenstein view 0.01580.0061 0.00430.0026 0.00530.0020 ‹0.001,††
Abbreviation: AP, anteroposterior; CoC: ceramic-on-ceramic; MoM: metal-on-metal; MoP: metal on highly cross-linked polyethylene
Femoral head penetration could not be measured for 8 joints in the CoC group and for 2 joints in the MoM group, because the margin of the femoral head could not be identiﬁed clearly in these joints. The wear rates were measured for 97 joints in the CoC group and for 53 joints in the MoM group.
All of the values are given as mean and standard deviation (SD).
‡CoC THAs vs MoM THAs:p<0.05 (95% conﬁdence interval [CI]: 0.00071–0.00292).
§CoC THAs vs MoP THAs:p<0.001 (95% CI: 0.01115–0.00137).
¶MoM THAs vs MoP THAs:p<0.001 (95% CI: 0.00934–0.01253).
CoC THAs vs MoP THAs:p<0.001 (95% CI: 0.00997–0.01268).
††MoM THAs vs MoP THAs:p<0.001 (95% CI: 0.00900–0.01221).
Fig. 3 Linear regression for mean femoral head penetration over time in the CoC THA and on the MoM and MoP THA groups. The slope and intercept are considered to represent true wear and creep, respectively. Abbreviations: AP: anteroposterior; CoC: ceramic-on-ceramic; MoM:
metal-on-metal; MoP: metal on highly cross-linked polyethylene.
Although CoC and MoM THAs had a lower wear rate than MoP THAs, the three types of THAs provided good implant survivorship. However, osteolysis among MoM THAs was more frequently observed compared with MoP and CoC THAs. Studies that span a longer follow-up period are needed to better understand the effects of wear rate and material bioactivity on implant longevity.
Conﬂicts of Interests
The authors have no conﬂicts of interests to declare.
1 D’Antonio JA, Capello WN, Naughton M. Ceramic bearings for total hip arthroplasty have high survivorship at 10 years. Clin Orthop Relat Res 2012;470(02):373–381
2 Shetty V, Shitole B, Shetty G, Thakur H, Bhandari M. Optimal bearing surfaces for total hip replacement in the young patient: a meta-analysis. Int Orthop 2011;35(09):1281–1287
3 Callary SA, Solomon LB, Holubowycz OT, Campbell DG, Munn Z, Howie DW. Wear of highly crosslinked polyethylene acetabular components. Acta Orthop 2015;86(02):159–168
4 D’Antonio J, Capello W, Manley M, Bierbaum B. New experience with alumina-on-alumina ceramic bearings for total hip arthro- plasty. J Arthroplasty 2002;17(04):390–397
5 Engh CA Jr, Stepniewski AS, Ginn SD, Beykirch SE, Sychterz- Terefenko CJ, Hopper RH, et al. A randomized prospective evalua- tion of outcomes after total hip arthroplasty using cross-linked marathon and non-cross-linked Enduron polyethylene liners.
J Arthroplasty 2006;21(06, Suppl 2):17–25
6 Nikolaou VS, Edwards MR, Bogoch E, Schemitsch EH, Waddell JP.
A prospective randomised controlled trial comparing three alter- native bearing surfaces in primary total hip replacement. J Bone Joint Surg Br 2012;94(04):459–465
7 Takao M, Ohzono K, Nishii T, Miki H, Nakamura N, Sugano N.
Cementless modular total hip arthroplasty with subtrochanteric shortening osteotomy for hips with developmental dysplasia.
J Bone Joint Surg Am 2011;93(06):548–555
8 Milošev I, KovačS, Trebše R, LevašičV, Pišot V. Comparison of ten- year survivorship of hip prostheses with use of conventional polyethylene, metal-on-metal, or ceramic-on-ceramic bearings.
J Bone Joint Surg Am 2012;94(19):1756–1763
9 Wyles CC, Jimenez-Almonte JH, Murad MH, Norambuena-Mor- ales GA, Cabanela ME, Sierra RJ, et al. There Are No Differences in Short- to Mid-term Survivorship Among Total Hip-bearing Sur- face Options: A Network Meta-analysis. Clin Orthop Relat Res 2015;473(06):2031–2041
10 Bascarevic Z, Vukasinovic Z, Slavkovic N, Dulic B, Trajkovic G, Bascarevic V, et al. Alumina-on-alumina ceramic versus metal- on-highly cross-linked polyethylene bearings in total hip arthro- plasty: a comparative study. Int Orthop 2010;34(08):1129–1135 11 Higuchi Y, Hasegawa Y, Seki T, Komatsu D, Ishiguro N. Signiﬁ- cantly Lower Wear of Ceramic-on-Ceramic Bearings Than Metal- on-Highly Cross-Linked Polyethylene Bearings: A 10- to 14-Year Follow-Up Study. J Arthroplasty 2016;31(06):1246–1250 12 Kanoh T, Hasegawa Y, Masui T, Yamaguchi J, Kawabe K, Ishiguro N.
Accurate acetabular component orientation after total hip arthro- plasty using an acetabular alignment guide. J Arthroplasty 2010;
13 Mestriner MB, Verquietini CM, Waisberg G, Akkari M, Fukunaga ET, Santili C. Radiographic evaluation in epiphysiolysis: possible predictors of bilaterality? Acta Ortop Bras 2012;20(04):
14 Kim YH, Kim JS, Oh SH, Kim JM. Comparison of porous-coated titanium femoral stems with and without hydroxyapatite coating.
J Bone Joint Surg Am 2003;85-A(09):1682–1688
15 Sutherland CJ, Wilde AH, Borden LS, Marks KE. A ten-year follow- up of one hundred consecutive Müller curved-stem total hip- replacement arthroplasties. J Bone Joint Surg Am 1982;64(07):
16 Lee JH, Lee BW, Lee BJ, Kim SY. Midterm results of primary total hip arthroplasty using highly cross-linked polyethylene: minimum 7-year follow-up study. J Arthroplasty 2011;26(07):1014–1019
17 Lewinnek GE, Lewis JL, Tarr R, Compere CL, Zimmerman JR.
Dislocations after total hip-replacement arthroplasties. J Bone Joint Surg Am 1978;60(02):217–220
18 Barrack RL, Lavernia C, Szuszczewicz ES, Sawhney J. Radiographic wear measurements in a cementless metal-backed modular cobalt-chromium acetabular component. J Arthroplasty 2001;
19 García-Rey E, García-Cimbrelo E, Cruz-Pardos A, Ortega-Cha- marro J. New polyethylenes in total hip replacement: a prospec- tive, comparative clinical study of two types of liner. J Bone Joint Surg Br 2008;90(02):149–153
20 Brooker AF, Bowerman JW, Robinson RA, Riley LH Jr. Ectopic ossiﬁcation following total hip replacement. Incidence and a method of classiﬁcation. J Bone Joint Surg Am 1973;55(08):
21 Cai P, Hu Y, Xie J. Large-diameter Delta ceramic-on-ceramic versus common-sized ceramic-on-polyethylene bearings in THA. Ortho- pedics 2012;35(09):e1307–e1313
22 Gallo J, Goodman SB, Lostak J, Janout M. Advantages and dis- advantages of ceramic on ceramic total hip arthroplasty: a review.
Biomed Pap Med Fac Univ Palacky Olomouc Czech Repub 2012;
23 Lombardi AV Jr, Mallory TH, Cuckler JM, Williams J, Berend KR, Smith TM. Mid-term results of a polyethylene-free metal-on- metal articulation. J Arthroplasty 2004;19(07, Suppl 2):42–47 24 Yin S, Zhang D, Du H, Du H, Yin Z, Qiu Y. Is there any difference in
survivorship of total hip arthroplasty with different bearing surfaces? A systematic review and network meta-analysis. Int J Clin Exp Med 2015;8(11):21871–21885
25 Greiner JJ, Callaghan JJ, Bedard NA, Liu SS, Goetz DD, Mahoney CR.
Metal-on-Metal Total Hip Arthroplasty at Five to Twelve Years Follow-Up: A Concise Follow-Up of a Previous Report.
J Arthroplasty 2016;31(08):1773–1778
26 Capello WN, D’Antonio JA, Ramakrishnan R, Naughton M. Con- tinued improved wear with an annealed highly cross-linked polyethylene. Clin Orthop Relat Res 2011;469(03):825–830 27 Reynolds SE, Malkani AL, Ramakrishnan R, Yakkanti MR. Wear
analysis ofﬁrst-generation highly cross-linked polyethylene in primary total hip arthroplasty: an average 9-year follow-up.
J Arthroplasty 2012;27(06):1064–1068
28 Epinette J-A, Manley MT. No differences found in bearing related hip survivorship at 10-12 years follow-up between patients with ceramic on highly cross-linked polyethylene bearings compared to patients with ceramic on ceramic bearings. J Arthroplasty 2014;29(07):1369–1372
29 Al-Hajjar M, Fisher J, Tipper JL, Williams S, Jennings LM. Wear of 36-mm BIOLOX(R) delta ceramic-on-ceramic bearing in total hip replacements under edge loading conditions. Proc Inst Mech Eng H 2013;227(05):535–542